Transparent polycrystalline alumina using spark plasma ... 6)2010.pdf¢ Transparent...
Embed Size (px)
Transcript of Transparent polycrystalline alumina using spark plasma ... 6)2010.pdf¢ Transparent...
d p d ©
Available online at www.sciencedirect.com
Journal of the European Ceramic Society 30 (2010) 1335–1343
Transparent polycrystalline alumina using spark plasma sintering: Effect of Mg, Y and La doping
Michael Stuer a,b, Zhe Zhao b,∗, Ulrich Aschauer a, Paul Bowen a a Powder Technology Laboratory, Material Science Institute, Swiss Federal Institute of Technology, CH-1015, Lausanne, Switzerland
b Department of Physical, Inorganic and Structural Chemistry, Arrhenius Laboratory, Stockholm University, SE-10691, Stockholm, Sweden
Received 7 July 2009; received in revised form 13 November 2009; accepted 1 December 2009 Available online 22 December 2009
ransparent polycrystalline alumina (PCA) is a promising replacement for sapphire. Its optical properties however are highly dependent on the rain size and residual porosity which need to be controlled for real inline transmittances (RIT), that are high enough for possible applications.
To achieve high RITs, doping as well as pressure assisted sintering is often used. In this study spark plasma sintering (SPS) and doping are nvestigated. A systematic experimental design is used to study the influence of Mg, Y and La single or co-doping (75–450 ppm) as well as the PS sintering pressure and temperature on the RIT and grain size of PCA. Using optimized sintering parameters, RITs of >50% were attained in the visible wavelength (640 nm) for 0.8 mm thick samples for almost all
oping strategies. The best RIT of 57% was for triple-doped samples at a total dopant level of 450 ppm. These results are significantly better than reviously published SPS studies and illustrate that SPS sintered alumina can attain high and reproducible optical transmittances under various oping and sintering conditions.
2009 Elsevier Ltd. All rights reserved.
Keywords: Al2O3; Sintering; Optical properties; SPS
Over recent years, attempts have been made to replace sap- phire by transparent polycrystalline alumina (PCA)1–6 for both economic and ecological reasons.
The most important parameters controlling the degree of transparency achievable for polycrystalline materials are the grain size (e.g. light scattering by grains γG)1 and the poros- ity (e.g. light scattering by pores γP)7 as can be seen from the model for the real inline transmittance (RIT) given by Eqs. (1)8
RIT = I I0
=(1 = RS)exp(−γtotD) (1)
tot=γG + γP + · · ·=3π 2r�n2
λ20 + 3VPQeff
4rmexp(3.5δ2) + · · · (2)
∗ Corresponding author. E-mail address: email@example.com (Z. Zhao).
955-2219/$ – see front matter © 2009 Elsevier Ltd. All rights reserved. oi:10.1016/j.jeurceramsoc.2009.12.001
with I0 and I the light beam intensities before and after travel- ling through a PCA sample with an apparent thickness D; RS the total normal surface reflectance (RS(Al2O3) = 0.14) and γ tot the total scattering (absorption) coefficient; γG and γP the scattering contributions from the grains and the pores, respectively; r the (average) grain radius; �n the (average) refractive index change between two adjacent grains (�nmax = no − ne = 0.008); λ0 the wavelength of the incident light in vacuum; Vp the specific pore volume; rm the radius of the mode of the pore size distribution; δ the standard deviation factor for a lognormal distribution and Qeff an effective dimensionless scattering efficiency of the pores. The simulated contributions of grains and pores on the RIT are illustrated in Fig. 1 and described more in detail elsewhere.1,7
This light scattering theory predicts the requirement of an aver- age grain size diameter below 250 nm and a density above 99.995 vol.% for PCA to be competitive with sapphire in terms of RIT in the visible range (PCA > 80%; sapphire = 86%).
Over the last decade, several groups have tried to produce
high-RIT PCA samples with two different strategies, namely natural sintering coupled with post-hot isostatic pressing (HIP) and spark plasma sintering (SPS).
1336 M. Stuer et al. / Journal of the European C
F a R
d b b K s s p g t r o s u c t d b m
h ( t f i H c p m h b
r t m s
dopant ratio as well as the dopant elements (M = magnesium,
ig. 1. Influence of grain size diameter, porosity (pore diameter 20 nm) and verage refractive index change according to the optical model (Eq. (1)) on the IT of PCA.
For post- HIP treated samples, results for undoped,5 single- oped (Mg2+, Ti4+)1,3,9 and co-doped (Ca2+–Ti4+)10 PCA have een reported so far. This method gave fairly reproducible RITs etween different groups with values up to 65%. However only rell et al. reached RITs as high as 72%.5 From some of these
tudies, it appeared that achieving “full” density without exten- ive grain growth can be favored by defect free green body rocessing.5,11 Defect free high density green body fabrication ives a more homogeneous porosity distribution. This allows he pores to close as late as possible during the sintering cycle, educes the sintering temperature5,11 and retards the occurrence f grain growth.12,13 As well as processing, the quality of the tarting powder also plays a key role. Due to the very limited sol- bility of ions in Al2O3 (in the ppm range), the grain boundary omposition can be affected by segregated dopants or impuri- ies, the powder should thus be of very high purity. Selective oping can further enhance densification versus grain growth y promoting densification and reducing the grain boundary obility.9,14,15
For spark plasma sintered PCA samples, reported results2,16
ave been less promising, with a maximum RIT of 35% λ = 640 nm, thickness 1 mm; calculated RIT of 40% for 0.8 mm hickness according to Eq. (3)).16 Reproducibility between dif- erent groups seems to be an issue and the achieved RITs are not n the range of those obtained with traditional sintering methods. owever, careful powder processing to avoid agglomeration or
ontamination as well as improvements of the SPS sintering arameters should help to show the benefits of SPS.17 Further- ore, in all the SPS studies reported to date the graphite dies
ave been loaded directly with the alumina powder (i.e. no green ody).
No systematic research has been reported concerning the fab- ication of doped polycrystalline alumina by SPS. In this study he effects of Mg, Y and La doping (single and combined) on the
icrostructure and light transmittance (i.e. RIT) of spark plasma intered PCA were systematically evaluated.
Magnesium has been chosen due to its effects on grain bound- ry/surface diffusion14,18 and grain boundary mobility,14,18 the eported surface roughening19,20 and its liquid scavenger19,21
eramic Society 30 (2010) 1335–1343
effects. It is expected to enhance densification (e.g. by lower- ing the activation energy), avoid abnormal or anisotropic grain growth as well as influence the atomic arrangement and thus potentially the dopant cation solubility in the grain boundary area (e.g. oxygen vacancies).
Yttria has mainly been reported to increase creep resistance of alumina and to hinder grain growth during sintering.22,23 It has a very low solubility in alumina and thus strongly segregates at grain boundaries24–26 where it hinders diffusion processes and causes solute drag to occur. Its effects on the diffusion processes might be linked to the recently reported pattern formation of Y atoms at specific grain boundaries.25
The larger cation size of lanthanum compared to yttria but identical valence leads us to expect La to have stronger effects than yttria. Although both inhibit densification and grain growth, La has been reported to be the better grain growth inhibitor whereas Y is the better densification inhibitor15 (c.f. pattern formation25).
The solubility of the selected dopants is very limited in alu- mina. The solid solution limits above which segregation or segregation plus precipitation occurs are commonly admitted to be in cationic ratios ([dopant]/[Al]) in the ppm range (for Mg < 200 ppm27 and for Y and La even lower).
Although the effects of these dopants have been extensively reported in the literature, their effect may be different due to changes in kinetics when using SPS, where sintering of pieces takes several minutes rather than hours for natural sintering. The aim of this work is to provide a basic approach to achieve reproducible high-RIT ceramics by SPS and to better evaluate its application for the production of transparent PCA.
2. Materials and experimental method
The powder used was a polyhedral near-spherical high purity �-Al2O3 with a median particle size Dv50 of 510 nm, a total impurity concentration of less than 0.01 mass% (≤5 ppm for Si, Na, Mg, Cu and Fe) and a specific surface SBET of 4.2 m2/g.
Doping was carried out by dispersing 25 g of the pow- der in 60 mL 0.01 M HNO3 and adding the required dopant solutions Mg(NO3)2·6H2O, Y(NO3)3·6H2O, La(NO3)3·6H2O (purity >99%, dissolved in 0.01 M HNO3) to achieve the desired cationic dopant ratio. After the dopant addition, 0.01 M HNO3 was added to reach a final volume of 80 mL. The suspension was stirred for 5 min and then treated for 10 min in an ultrasonic bath. The suspension was then frozen in liquid nitrogen and freeze- dried during approximately 45 h (−50 ◦C @ 0.08–0.1 mbar, Alpha 1-4, Christ, Germany).
All single, double and triple dopant combinations of the 3 dopants Mg, Y and La were prepared for a total cati